Micro- and Nano- encapsulation of Water- and Oil-soluble ... 17 Micro- and Nano-encapsulation of Water- and Oil-soluble Actives for Cosmetic and Pharmaceutical Applications David Fairhurst, PhD and Andrew ...
Post on 06-Feb-2018
Embed Size (px)
<ul><li><p>Chapter 17</p><p>Micro- and Nano-encapsulation of Water- and Oil-soluble Actives for Cosmetic and Pharmaceutical ApplicationsDavid Fairhurst, PhD and Andrew Loxley, PhD</p><p>Particle Sciences Inc., Bethlehem, PA, USA</p><p>Abstract</p><p>Skin, hair and mucosal surfaces are useful targets for the delivery of active compounds, botanicals and, importantly, drugs. Encapsulation provides an invaluable tool to the cosmetic and/or pharmaceutical formulator, providing great flexibility in the choice of delivery mechanisms and excipients that can be used. Dispersions of solid lipid nanoparticles (SLNs) were prepared using biodegradable materials generally regarded as safe by a melt-emulsify-chill (MEC) method. Among the materials encapsulated in SLNs were hydropho-bic active pharmaceutical ingredients, antiviral and fungicidal compounds, organic UV absorbers and fluorescent dyes. The loading, adhesion and intra-cellular localization of the SLNs were studied as a function of surface charge. </p><p>The MEC process can easily, and cheaply, produce a range of solid lipid nanoparticles (SLNs) - smart colloids - that offer flexibility in formula-tion, increased efficacy and decreased formulation complexity. The method is general and can be applied to many water- or oil- soluble cosmetic and pharmaceutical actives. Multiple actives can be co-encapsulated. The process is cost-effective, reproducible, robust and scalable. The bulk physi-cal characteristics and surface chemical properties can be varied to allow systems to be custom designed to fit specific applications; use can be made </p></li><li><p>Cosmetic Delivery Systems Micro- and Nano-encapsulation</p><p>24</p><p>of this in the targeting of encapsulated actives, botanicals and therapeutics to skin and hair.</p><p>The non-specific nature of cellular uptake would suggest that SLNs produced via the MEC process are suitable candidates for delivering surface-attached actives into cells. The strong attachment and demonstrated entry into antigen presenting cells of the immune system illustrates the potential that these natural wax nanoparticles might have in vaccine formulations. </p><p>17.1 IntroductionSkin, hair and mucosal surfaces are useful targets for the delivery of active compounds, botanicals and, importantly, drugs. Encapsulation provides an invaluable tool to the cosmetic and/or pharmaceutical formulator, providing great flexibility in the choice of delivery mechanisms and excipients that can be used. For example, active pharmaceutical ingredients can be delivered in systems that would otherwise be unacceptable or hostile to them. Lipophilic (??) active compounds can be incorporated into aqueous dispersions without the need for a solvent. Conversely, water-soluble ingredients can be deliv-ered in non-aqueous systems such as ointments. The matrix of the capsule can be chosen from a wide variety of materials (usually selected from a list of materials generally regarded as safe (GRAS) for pharmaceutical applica-tions) to meet the needs of the application as well as regulatory demands, e.g., biodegradability. Multiple actives can also be delivered in the same particle; indeed, mutually chemically incompatible actives can be formulated together. A further way to exploit this technology is to encapsulate one ingredient that can facilitate, or stabilize, a second. By isolating problematic ingredients, formulation and processing issues are minimized; undesirable properties can be masked. This chapter is a brief review of traditional encapsulation meth-ods that will be helpful as the basis for further discussing other encapsulation technologies.</p><p>17.2 MicroencapsulationConventional microencapsulation can be described as surrounding either a liquid droplet or a solid particle core with a defined, solid shell (see Fig-ure 17.1). It is used to deliver, protect, stabilize or control the release of the core. Ingredients so encapsulated include adhesives, drug substances, colors, fragrances, flavors, agricultural chemicals, solvents and oils. Especially in the cosmetic industry such capsules are designed to release the core by fracture of the shell. Although the earliest application by the cosmetic industry was probably for scratch and sniff fragrance samplers, the first commercial use </p></li><li><p>David Fairhurst et al. Chapter 17 </p><p>25</p><p>of microencapsulation was in carbonless paper.1,2Traditional microencapsulation capsules are typically larger than 1 m in </p><p>diameter, the normal range being 50500 m. Capsule size is determined, in part, by limitations of the methods used to produce them and by the fact that a large size is necessary for the capsule to be ruptured by either pres-sure or by shear of use. As capsule size decreases the capsules become less susceptible to the forces that can cause rupture of the shell. Such capsules are normally supplied in a dry powder form that, subsequently, often needs to be </p><p>Figure 17.1. Schematic comparing microcapsules with SLNs.</p></li><li><p>Cosmetic Delivery Systems Micro- and Nano-encapsulation</p><p>26</p><p>incorporated (dispersed) into the cosmetic or pharmaceutical formulation.</p><p>17.3 Chemical ProductionMicroencapsulation capsules are produced by chemical or physical processes. The chemical methods used are categorized as coacervation, con-densation or interfacial polymerization and generally involve dispersing the active core material in a non-solvent continuous phase to form an emulsion or dispersion (the continuous phase must be a non-solvent for the dispersed phase). The shell is created by a chemical reaction, and subsequent precipi-tation, of one or more shell-precursor materials that are dissolved in the continuous or discontinuous, phase at the interface of the core material and the continuous phase. It is possible to have different components of the shell dissolved in both phases.</p><p>Microcapsules prepared by coacervation rely on the fact that oppositely charged (natural and synthetic) polymers condense in solution and can attach to the surface of an emulsified oil droplet (see Figure 17.2). In coacer-vation encapsulation, a shell material precursor is normally dissolved in the continuous phase. Classic shell materials used are gelatin or Arabic gum dissolved in an aqueous continuous phase. Varying the conditions of the continuous phase, either by altering the pH or by adding a water-miscible solvent, changes the solubility of the dissolved shell material. This change in solubility causes the shell material to migrate to the surface of the dis-persed core and to coat the non-continuous droplets. Another material is then added to chemically crosslink the shell material thus forming a hard shell around the active core.3-5 The capsules can be as small as a few microns in diameter, or as large as a few millimeters. In this way, a wide range of encapsulated products can be produced where the encapsulation provides flavor-masking, payload degradation protection, or simply for the case where a liquid needs to be handled more as a solid (the dried capsules can be handled as a powder and the liquid contents evaporate only very slowly).</p><p>An alternative technique uses the phase separation of polymers in poor solvents to allow preparation of microcapsules from a wide range of hydro-phobic polymers, such as poly(methylmethacrylate)Plexiglass.6 Using this method, and utilizing polymers that change their properties with pH, microcapsules with pH-controlled release of model marker compounds can be prepared. Shown in Figure 17.3 is an SEM of a microcapsule made with a shell of poly (4-vinylpyridine)a material that swells at about or below pH 4. Figure 17.4 shows the pH-dependent release kinetics for a marker compound dissolved within the core. The first order release of the encap-sulated material was faster at a pH below the polymer swelling pH (solid </p></li><li><p>David Fairhurst et al. Chapter 17 </p><p>27</p><p>Figure 17.2. Optical micrograph of gelatin-acacia microcapsule prepared by coacervation.</p><p>Figure 17.3. SEM of fractured poly(4-vinylpyridine) microcapsule.</p></li><li><p>Cosmetic Delivery Systems Micro- and Nano-encapsulation</p><p>28</p><p>Figure 17.4. pH dependent release kinetics from a PVPy microcapsule</p><p>symbols).Condensation and interfacial polymerization methods entail polym-</p><p>erization or cross-linking at the continuous/non-continuous interface of monomer or components dissolved in one or more phases.7 The dispersion of capsules may be dried to provide a powder. Shell materials commonly used include polyesters, polyurethanes, polyureas, polycyanoacrylates and melamine-formaldehyde resins. Materials used to form, cross-link or harden the shell must be screened for any unwanted reaction with the core ingre-dients as well as for their toxicological potential; residual monomer content can pose a problem as is the presence of residual solvent.</p><p>17.4 Physical ProductionThese methods entail co-extrusion of a solution, melting the shell material over a droplet, or particle, of the core material, or spray-coating the shell over a solid particle where fluidized beds are often employed to ensure uniform coating of cores by shell forming solutions. The Wurster Process is the classic example, in which particles are fluidized in an air stream within a vertical chamber and coating material solution is injected from below into the fluidized particles. Such physical methods typically produce larger capsules, and are especially suited to particles with solid cores. For more </p></li><li><p>David Fairhurst et al. Chapter 17 </p><p>29</p><p>details on this process, see Chapter 18, Encapsulation and Other Topical Delivery Systems.</p><p>17.5 LiposomesLiposomes are a special case of microencapsulation. However, since the typical liposomal particle size is around 200 nm such systems should more rightly be termed sub-microcapsules or nanocapsules. Liposomes are self-assembled spherical micro-structures of lipids and lipid-like amphiphilic molecules that are arranged in single or multilayered closed bilayers in aque-ous media; the active is trapped inside this fatty wall or the aqueous core. Since the wall material comprises triglycerides and phospholipids, when used in topical delivery liposomes can facilitate absorption of the active into the epidermis; the liposomes, themselves, do not appear to penetrate intact into the skin.8 Although liposome technology has been around for about 40 years, it has suffered from problems of stability, poor mechanical integrity and low active concentrations.9 Ever since the invention of liposomes, con-tinuing efforts have been aimed at achieving a better understanding of lipid properties in order to gain better control over liposome formation and use. Their use in cosmetics has been extensively reviewed.10 For more details, see Chapter 15, Flexible Liposomes for Topical Applications in Cosmetics.</p><p>These issues have been addressed with the recent advent of the so-called micellar nanoparticlesmulti-lamellar structures that are liposome-like.11 Here, the outer layer encases the water containing the active pharmaceutical ingredient that allows delivery of the active to the interior of the epidermis.</p><p>17.6 Solid-Lipid NanoparticlesParticulate lipid matrices, in the form of lipid pellets were originally devel-oped for oral drug administration.12 Solid-lipid nanospheres were initially produced by high pressure homogenization of melted or solid lipids.13 Our work in this area began with the preparation and scale up of SLNs by a solvent-free process for the encapsulation of ethylhexyl methoxycinna-mate (EHMC; Octinoxate) for dermal sunscreens.14 Initially, the goal was to encapsulate the organic sunscreen in a benign matrix and effectively turn them into particulates in order to decrease the irritant/allergic sensitization potential. A low pressure proprietary melt-emulsify-chill (MEC) process was used (see Figure 17.5). This encapsulation method is general and can be applied to many water- or oil-soluble cosmetic and pharmaceutical actives. The process is cost-effective, reproducible, robust and scalable. For economic and technical (processing) reasons, it is very desirable to have a high solids-</p></li><li><p>Cosmetic Delivery Systems Micro- and Nano-encapsulation</p><p>30</p><p>content particle dispersion; stable, concentrated aqueous dispersions (up to 60% w/w) of SLNs can be prepared by the MEC method. The particle sizes range from 0.11 m (see Figure 17.6); in the example shown the mean particle diameters were between 300 and 400 nm. The particle size and dis-tribution is controlled by the rate of initial mixing, degree of shear and rate of cooling. These particles are a homogeneous mixture of matrix and active; the active can be present at concentrations as high as 30% by weight of the total dispersion. The matrix is typically a wax (or mixture of waxes) but may </p><p>Figure 17.5. Schematic of the Melt-Emulsify-Chill process.</p></li><li><p>David Fairhurst et al. Chapter 17 </p><p>31</p><p>Figure 17.6. SEM of a typical SLN. Note that the particles are spherical but polydisperse.</p><p> Table 17.1. Controllable particle parameters using the Melt-Emulsify-Chill process</p><p>Bulk Physical Characteristics Surface Chemical PropertiesMelting point, hardness, density, solubility Surface charge (anionic, nonionic, cationic)Particle size and distribution Hydrophobic/Hydrophilic BalanceBioadhesion Polarity </p><p>be an organic polymer or a silicone. A list of the controllable particle param-eters are given in Table 17.1. In principle, the MEC process allows systems to be custom-designed to fit specific applications.</p><p>The SLN is not a wall-and-core particle; the particles are stable to mechanical agitation as well as storageunlike many liposomal systems. Release is accomplished via diffusion or particle breakdown. Diffusion is dependent on particle/surrounding medium interaction. Breakdown can be accomplished through exploitation of melting points. For example, an </p></li><li><p>Cosmetic Delivery Systems Micro- and Nano-encapsulation</p><p>32</p><p>active could be released in a matrix that melts or softens at body tempera-ture or, an orally ingested drug could be encapsulated in a polymer that dissolves at stomach pH.</p><p>The MEC process has now been extended to the encapsulation of other hydrophobic and hydrophilic molecules, specifically to prepare biodegrad-able nanoparticles as carriers for drugs. We have investigated the attachment of a model antigen-tetanus toxoid (TTA) and the effect of surface charge on the adhesion of SLNs to cells and tissues. The TTA was electrostatically adsorbed to the surface of cationic SLNs. Cationic SLNs were also found to adsorb strongly to human hair shafts, making them useful for time-release of drugs from the hair, or to the surface of hair-bearing skin. SLN formulations containing encapsulated fluorochromes were efficiently internalized by anti-gen presenting cells of the immune system in vitro, making them interesting candidates as sub-unit vaccine carriers for mucosal vaccination.</p><p>17.7 Experimental MethodsSolid lipid nanoparticles were prepared by the MEC process as shown in Fig-ure 17.5. In essence, a molten wax is dispersed into a hot aqueous emulsifier solution under controlled sh...</p></li></ul>
View more >
Coaxial electrospinning for encapsulation and controlled release of fragile water-soluble bioactive agents
ChemInform Abstract: Water-Soluble Octahedral Polyammonium Nanocapsules: Synthesis and Encapsulation Studies.
MICRO NANO encapsulation - swri.org ?· Practices-compliant laboratory for encapsulation studies related…
Nano and Micro Particles in Water and Wastewater ?· Nano and Micro Particles in Water and Wastewater…
Instantaneous enteric nano-encapsulation of omeprazole: Pharmaceutical and pharmacological evaluation
Micro- and Nano-encapsulation Technologies - ?· Micro- and Nano-encapsulation Technologies ... Oregano,…
Direct encapsulation of water-soluble drug into silica microcapsules for sustained release applications
Water Soluble Star-block Copolypeptides: Towards Biodegradable Nanocarriers for Versatile and Simultaneous Encapsulation